HIGH-ENERGY, HIGH-DOSE O IMPLANTATION IN Si
Susan Leigh Ellingboe
A Thesis Submitted for the Degree of
DOCTOR OF PHILOSOPHY
AUSTRALIAN NATIONAL UNIVERSITY
Research School of Physical Sciences and Engineering
I certify that this thesis does not incorporate without acknowledgment, any material
previously submitted for a degree or diploma in any university; and that to the best of
my knowledge and belief it does not contain any material previously published or
I would like to extend my sincere thanks to my supervisor, Dr. Mark Ridgway for providing a role model of the kind of scientist I want to be. He was a continual source of support and guidance throughout my PhD. work. Appreciation is also given to my co-advisors, Dr. Jim Williams and Dr. Robert Elliman, and to Dr. C. Jagadish for providing an atmosphere conducive to doing “good” science and for teaching me good scientific practices.
The Australian Defence Force Academy is gratefully acknowledged for the use of their TEM. All of the TEM work in Chapter 3 was performed on their equipment. Dr. Van Watenaar and John Malunec are thanked for sharing their knowledge of electron microscopy as well as providing technical support. The TEM work in Chapters 4 and 5 was performed at the Electron Microscopy Unit in the Research School of Biological Sciences at the ANU. David Llewelyn, Alan Lee and Dr. Sally Stowe are acknowledged for technical support. For help in TEM micrograph interpretation, I extend my thanks to Dr. John Fitz Gerald. Dr. Peter Schultz and Dr. P. Simpson of the University of Western Ontario are acknowledged for providing VEP measurements on SIMOX samples.
Bemie King, Tom Halstead, Marco Maldoni, Tony Watt and Alan Hayes provided technical support and guidance that is much appreciated. They are all thanked for inadvertently giving me lessons on the Australian male.
Thanks for proof reading go to Dr. Renate Egan, John Glasko, and Dr. Mark Ridgway. The small favours by John Glasko after the author left Australia are especially appreciated. Andrew Clark deserves a special acknowledgment for being a best friend at and outside of work. Jennifer Wong-Leung, Dr. Renate Egan and Franca Placidi provided a support network of female colleagues and are thanked for many enjoyable conversations. My fellow students at EME made my work more enjoyable and were constant sources of information and help. They include W.C. Wong, Kidane Belay, Andrew Clark, Jennifer Wong-Leung, Hoe Tan, John Glasko and Paul Gortmaker.
Special thanks to Mark Jamyk and Judy Kay for having more faith in me than I had in myself at times. Thanks to my family (mom, dad, Kathy and Megan) for their continual support. For inspiring me to be all that I can be I thank my grandfather, Sylvester Thomas.
High-energy, High-dose O Implantation in Si
The formation of Separation by Implantation of Oxygen (SIMOX) material by MeV O-ion implantation was investigated at doses between 0.3-2.18x10 O/cm . It was demonstrated that implant temperatures as low as 150°C can be used for SIMOX fabrication without total amorphisation of the Si overlayer. The microstructure of the material after annealing was found to be highly implant-temperature dependent, with lower implant temperatures (~150°C) suppressing Si02 and Si precipitate formation within the Si overlayer and buried Si02 layer, respectively. MeV self-ion implantation in Si was performed to elucidate the contribution of a high O impurity concentration to damage formation in high-dose O-implanted Si. It was shown that a high O concentration contributes to amorphous layer formation at the ion end-of-range. Conversely, a comparison of O and Si implantation at doses which produced a similar athermal vacancy concentration at depths less than the ion end-of-range indicated that damage within the Si overlayer was independent of the implanted specie.
Tensile strain at depths less than the ion end-of-range in high-dose Si- and O-implantation was shown to be the result of an implantation-induced vacancy excess. The magnitude of the strain was related to implanted ion dose, implant temperature, and post-implantation annealing time. It was shown that when the strain maximum exceeds the yield strain of Si, dislocation formation results at the depth of the strain maximum. MeV O implantation was utilised to characterise, for the first time, the yield strength of Si between 150 and 450°C.
Table of Contents
Chapter 1: Introduction to Silicon-on-Insulator Process and
Technology1.0 Introduction... 1
1.1 Methods of Forming Silicon-on-Insulator Materials 1.1.1 Epitaxial Growth of Si on an Insulator... 2
1.1.1a Heteroepitaxial Techniques... 2
1.1.1b Homoepitaxial Techniques... 3
1.1.2 Full Isolation by Porous Oxidised Si (FIPOS)... 4
1.1.3 Recrystallisation Techniques... 5
1.1.4 Zone Melt Recrystallisation (ZMR)... ,...,.... 7
1.1.5 Wafer Bonding and Etch back... 8
1.2 SIMOX to Form SOI Material 1.2.1 History of SIMOX Material Fabrication... 10
1.2.2 Dependence of Damage on Oxygen Dose... 11
1.2.3 Dependence of Damage on Implant Temperature... 12
1.2.4 High-Temperature Annealing... 14
1.3 Refinements of the SIMOX Process to Form Low Defect Density SOI Material 1.3.1 Channeled Implants... 16
1.3.2 Si Epitaxial Growth on SIMOX substrates... 17
1.3.3 Cavity Nucleation in the Si overlayer... 18
1.3.4 Multiple Implantation and Annealing... 18
1.3.5 Low-Dose, Low-Energy SIMOX... 19
1.4 Scope of the Present Work... 19
Chapter 2: Experimental Techniques2.0 Introduction... 21
2.1.2 Furnace Annealing... 25
2.2 Sample Characterisation 2.2.1 Rutherford Backscattering... 26
2.2.2 Transmission Electron Microscopy 2.2.2a Operation... 28
2.2.2b Sample Preparation for Cross-Sectional TEM (XTEM)... 30
2.2.3 Double Crystal X-Ray Diffraction (DCXRD)... 31
2.2.3a Depth Distribution of Strain in Ion-implanted Material... 33
2.2.3b Rocking Curve Analysis by Dynamical Simulation (RADS).. 35
2.2.3c Strain Depth Profiling in Ion-Implanted Material... 35
2.4 Variable Energy Positron Annihilation Spectroscopy (VEP)... 40
Chapter 3: SIMOX Substrate Formation by High-Energy O-ion
Implantation3 0 Introduction... 42
31 High-Energy O-ion Implantation 3.1.1 Dependence of Damage on Dose... 43
3.1.2 Dependence of Damage on Implant Temperature... 46
3.1.3 Anneal Temperature and Time Dependence... 58
3.1.4 Discussion... 62
12 High-Energy Si-ion Implantation... 63
3.2.1 Experimental Results... 64
3.2.2 Discussion... 68
13 Conclusions... 69
Chapter 4: Damage and Strain Accumulation in O- and
Si-implanted Si•.0 Introduction... 71
•. 1 Strain in O- and Si-implanted Si 4.1.1 O-Implanted Si... 72
4.1.2 Si-Implanted Si... 79
4.2 Strain in O-Implanted Si; a Temperature Study
4.2.1 Experimental Results... 91
4.2.2 Discussion... 95
4.3 Conclusions... 100
Chapter 5: Damage Reduction in Strained and Strain-Relaxed
O-implanted Si by a Secondary Si Implant5.0 Introduction... 102
5.1 Si Implantation into Strained O-implanted Si 5.1.1 Strain Reduction by Si Implantation to Various Depths... 104
5.1.2 Dependence of Strain Reduction on Si Dose and Implant Temperature... 106
5.1.3 Discussion... 109
5.2 Si Implantation into Strain-Relaxed O-implanted Si 5.2.1 Dependence of Damage Micro structure on Si D ose... 113
5.2.1a Pre-anneal Microstructure... 113
5.2.1b Post-Anneal Microstructure... 115
5.2.2 Dependence of Damage Microstructure on Si Implant Energy... 118
5.2.3 Discussion... 120
5.3 Conclusions... 123
Chapter 6: Summary and Conclusions6.0 Summary and Conclusions... 125
Introduction to the Silicon-on-Insulator Process and
SOI substrate CMOS inverter
Figure 1.1: Schematic o f a typical device (CMOS inverterj fabricated on an SO I substrate.1
There are several methods of SOI substrate fabrication. A brief introduction to several of these technologies follows in section 1.1. Section 1.2 describes in more detail the method used for SOI substrate fabrication in this work, Separation by IMplantation of OXygen (SIMOX). At present, this is the leading and most commercially advanced technique. Finally, section 1.3 reviews the various processing methods used to improve
SIMOX material quality.
1.1 Methods of Forming Si-on-Insulator Materials
1.1.1 Epitaxial growth o f Si on an insulator
1.1.1a Heteroepitaxial techniques
Si substrate. Some examples of the latter include CaF2 and cubic zirconia. The choice of the insulator is governed by differences in lattice constant and thermal expansion coefficient (a) relative to Si. The Si epitaxial growth is typically performed at ~1000°C and, upon cooling, differences in a can increase lattice mismatch yielding strain and/or defect generation in the Si film. Unfortunately, is typically 2-3 times greater than a Si Thus, thermal mismatch is generally the most important factor determining the physical and electrical properties of heteroepitaxial Si films grown on insulators.
Si-on-sapphire (SOS) is the most common heteroepitaxial SOI materials system and the only one to reach production. (Wafers have been commercially available since 1971.) To produce SOS substrates, a Si film is deposited using the pyrolysis of silane at temperatures between 900-1000°C. The difference in thermal expansion coefficients (a Al203 - 2.5asi) results in high defect concentrations. Typical defect densities are 10 planar defects/cm and 10 line defects/cm . Although devices are fabricated on SOS material at present, this technology has several disadvantages. These not only include large defect densities but high production costs, mechanical fragility and the need for a dedicated A120 3 processing line. For a comprehensive review of SOS technology, see Gupta, et al.3,4
1.1.1b Homoepitaxial techniques
Figure 1.2: Schematic o f Epitaxial Lateral Overgrowth (ELO) using a seeding window2
A second technique is Lateral Solid Phase Epitaxy (LSPE) where lateral epitaxial growth of crystalline Si (c-Si) is accomplished through the controlled crystallisation of amorphous Si (a-Si). Amorphous Si is either deposited directly or polySi is amorphised using Si self-implantation. Seeding windows are again used to provide the template necessary for single-crystal growth. To suppress random nucleation in the a-Si, low recrystallisation temperatures (~600°C) are necessary. The major advantage of this technique is low-temperature processing. Disadvantages include residual defects in regions where two recrystallisation fronts intersect.
1.1.2 Full Isolation by Porous Oxidised Si (FIPOS)
Silicon nitride Thermal oxide
'X / / / / / S 7 ?
Figure 1.3: The FIFOS process, from left to right: formation o f n islands and p current paths, formation o f porous Si and oxidation o f the porous Si.5
oxidation since the oxidation rate of porous Si is orders of magnitude higher than c-Si. Upon oxidation, a thick buried oxide is formed while only a thin thermal oxide grows at the edges of the n -Si islands. The thermal oxide provides an interface of good structural and electrical quality between the Si and buried Si02.
Thin film applications are limited by non-uniformities introduced by the cusp where the anodisation fronts meet below the Si islands. As well, the requirement of a masking step to form Si islands hinders the commercialisation of the FIPOS process.
1.1.3 Recrystallisation techniques
underlying S i0 2. The recrystallisation o f a Si film on an insulator can be accomplished by irradiation with a laser and/or electron beam.
With the former, a continuous-wave Ar+ laser is typically utilised given the extent
o f absorption in Si at this wavelength. The beam is generally raster scanned over the entire wafer to induce local melting o f the Si. The scanned laser beam is ~50-150 pm in diameter and scan times are the order o f seconds. Recrystallisation o f the quenched Si proceeds along the thermal gradient produced by the laser. The beam shape (Gaussian) leads to undesirable thermal gradients along the recrystallisation path and small random crystallites due to thermal variations over the extent o f the irradiated area can result. These variations, which lead to thermal stress across the wafer during recrystallisation, are minimised by substrate preheating (~300-600°C). The recrystallisation proceeds laterally, beginning at a seeding window as shown in Figure 1.4. Upon melting, the reflectivity o f Si abruptly increases reducing the risk o f overheating. The use o f an
encapsulating layer (usually Si oxynitride) not only prevents delamination but is essential to minimise surface non-planarity. However, the production o f thin Si films is
difficult since a surface roughness o f >200 Ä is unavoidable.6
(100) silicon substrate
Recrystallisation of polySi films using an electron beam (e-beam) is similar to recrystallisation using a laser beam. Common seeding techniques are utilised and an
encapsulation layer is again necessary to prevent delamination of the molten Si. However, e-beams have the advantage that they can be scanned using electrostatic deflection which is far more flexible than scanning techniques used with laser beams.
1.1.4 Zone-Melt Recrystallisation (ZMR)
One of the disadvantages of laser and e-beam recrystallisation is the small molten zone produced by the beam that results in long processing times. Incoherent light is an alternative heat source which is used for ZMR. As schematically shown in Figure 1.5, a graphite strip or line-focused lamp can be passed over a Si wafer creating a molten zone along the length of the wafer.8 As a result, recrystallisation of an entire wafer can be accomplished in a single scan. The Si wafer (usually capped successively with Si02/polySi/Si oxynitride, the latter at the surface) is situated on a graphite susceptor. The susceptor is heated to within ~200°C of the Si melting temperature during the zone melting process and additional heating of the Si is produced locally at the surface of the wafer. Consequently, the thermal gradient across the wafer is much smaller than for the laser or e-beam technique. As with the aforementioned techniques, ZMR results in a recrystallised-Si surface non-planarity of -200 A.
Heated graphite susceptor
1.1.5 Wafer Bonding and Etch back
Theoretically, wafer bonding should yield a superior Si overlayer (i.e. a lower defect density) in comparison with the techniques previously described. As a consequence, there is great interest in this technique and wafers have recently become commercially available. There are four basic steps in this process as depicted in Figure 1.6. First, an etch stop (formed by implantation or epitaxy) or a polish stop (consisting of an embedded layer of slow polishing materials such as Si02) is produced. Then, two oxidised wafers - the device wafer (seed) and the handle wafer (handle) - are bonded together by placing the two hydrophilic Si02 surfaces against one another. Once initiated, the bonding process can spread in the form of a contacting wave with the speed of several cm/sec.9 Contacting forces are believed to be caused by the attraction of hydroxyl groups (OFF) adsorbed on the two surfaces. The bond between the two wafers is then strengthened by annealing at temperatures >800°C. Finally, the device wafer is thinned to the required overlayer thickness by one of two methods.
Etch stop formed
AWWWWWWWWWWWV i \ \ \ \ \ \ \ \ \ \ \ \ \ \ \ \ \ \ \ \ \ \ \ V +
Thin and etch back
s i0 2--- *
Final SOI wafer
1.2 SIMOX to form SOI Material
Although each of the previously discussed techniques of producing SOI material has certain advantages, SIMOX fabrication is the leading technology at present as a result of the inherent control of the Si overlayer thickness and compatibility with existing Si manufacturing processes. The electrical and mechanical properties of the Si overlayer are inferior to bulk Si, but satisfy the majority of microelectronic quality specifications. SIMOX substrates are commonly available up to 8" diameter with dislocation densities of < 10 cm' . The following sections give a brief history of SIMOX fabrication and discuss the parameters which determine the quality of SOI material fabricated with this technique.
1.2.1 History o f SIMOX Material Fabrication
1.2.2 Dependence o f Damage on Oxygen Dose
SIMOX is a high-dose process. While most implantation processes for the microelectronics industry require doses of < 10 cm* , SIMOX fabrication can necessitate doses of ~2xl018 O/cm2. To form stoichiometric Si02 during implantation, two O atoms are required for every Si atom. Thus, to form 4000Ä of Si02, a dose of
(Psio2 )(* S i0 2 )
2 O atoms molecule
, _22 molecules.,. ,
(2.27x1022 --- -— )(4xl0 5 cm)(2) 1.82x10'*
is required (assuming complete encorporation of O into the Si02 layer). Figure 1.7 shows the O depth distribution as a function of O dose as simulated using PROFILE code. Below the stoichiometric dose, the profile is approximately Gaussian. When the O concentration reaches 67 atomic %, Si02 forms and further implantation of O does not increase the peak O concentration but rather broadens the O profile (i.e. the buried oxide layer increases in width due to the rapid O diffusion in Si02).21
200 keV 1 MeV
Corresponds to 67 M 0
Figure 1.8 schematically depicts the evolution of damage with increasing dose during implantation. The swelling at the surface occurs because (1) an Si02 molecule occupies 2.2 times the volume of a Si atom, (2) the density of amorphous material is less than that of crystalline Si and (3) due to the addition of a high concentration of O atoms. The damage in the Si overlayer results from ion-induced atomic displacements, where at such doses each substrate atom is displaced from a lattice site hundreds or thousands of times. Such displacements (excluding replacement events) result in Frenkel pair generation:
Si <=> Si, + V (1.1)
(where I denotes an interstitial atom and V denotes a vacancy) when the post-collision energy of both atoms exceeds the displacement energy. The athermal depth distribution of implantation-induced disorder typically has a maximum at -0.8 Rp where Rp is the projected range of the implanted ion.
Since O is in a lower free-energy state in the form of Si02 than as an interstitial in a Si lattice (assuming the O concentration is in excess of the solid solubility), Si02 precipitates form during implantation. This internal oxidation process is another source
of point defects. The reaction yielding Si02 precipitation can be written as:
20j + xSi = Si02 + (x-l)Si] (12)
where x is any number of Si atoms. Oxidation thus results in the emission of Si interstitials and such point defects play a major role in the evolution of the disorder microstructure during both implantation and annealing. The annihilation of Si interstitials and vacancies can result from recombination or annihilation at the sample surface. Furthermore, large excesses of point defects can generate stacking faults, clusters or dislocations. These defects can pin O atoms and Si02 precipitates subsequently nucleate.
1.2.3 Dependence o f Damage on Implant Temperature
the effect of implant temperature on the defect depth distribution of 200 keV O-implanted Si. At very low temperatures (<300°C), the entire Si overlayer is amorphised yielding polySi upon annealing. Between 300 and 500°C, crystallinity in the Si overlayer is maintained but amorphisation has occurred near the front Si/Si02 interface. Since O impedes solid phase epitaxy, upon annealing the recrystallised Si at such depths is often twinned. In addition, point defects tend to cluster and form dislocation networks which are stable to very high annealing temperatures. At higher implant temperatures (>500°C), O-rich amorphous platelets embedded in highly damaged Si result near the ion end-of-range. Crystallinity in the Si overlayer is maintained at implant temperatures in excess of 500°C due to dynamic annealing. Higher implant temperatures result in a lower O concentration in the Si overlayer due to a greater redistribution of O atoms towards the peak of the O concentration.25 At very high implant temperatures (>800°C), Si02 precipitates begin to nucleate within the Si overlayer. Due to the extremely low diffusivity of Si in Si02 (~10*20 cm^/sec at 1000° C)26 these Si02 precipitates impede the flow of Si interstitials to the Si surface and consequently, the defect concentration increases.
Defective silicon overlayer
Increased oxygen dose
The implantation temperature also affects the uniformity of the buried oxide. Si trapped within the amorphous zones of Si02 results in the formation of Si precipitates within the buried Si02 layer upon annealing. At low implant temperatures (150°C), the size of the Si precipitates is decreased.27 These Si precipitates degrade electrical performance since they provide conductive paths between the Si overlayer and substrate.
Implantation temperature (9C)
Figure 1.9: Evolution o f damage in S1MOX material as a function o f implant temperature at a dose o f 1.8x10'8 cm’2 and an energy o f 200 keV.21
1.2.4 High-Temperature Annealing
Si + S i0 2
Damaged Si Si overlayer
Si substrate Silicon islands
Figure 1.10: Evolution o f SIMOX microstructure during high temperature annealing (A) as-implanted (B) 2 hr. at 1150°C (C) 6 hr. at 1185°C (D) 6 hr. at 1300°C.2i
can be explained by the thermodynamics of the Si-O system. Smaller precipitates are dissolved in favour of larger ones and the entire process is driven by tree-energy considerations. A critical precipitate radius (rc), below which Si02 precipitates will dissolve, can be defined as:
precipitate is stable and grows. At high temperatures the critical radius approaches infinity and a buried oxide layer (essentially a precipitate of infinite radius) is the only stable precipitate. While high-temperature annealing is essential to produce device grade SIMOX material, defects which have formed within the Si overlayer before post implantation annealing, such as threading dislocations and stacking faults, can not be totally eliminated by such annealing.
1.3 Refinements of the SIMOX Process to form Low-Defect-Density
In 1985 Jassaud, et al reported that post-implantation annealing at high temperatures (>1300°C) would rid the Si overlayer of Si02 precipitates. This high temperature annealing led to vast improvements in the Si/Si02 interface, but still left an unacceptably high density of dislocations (~10 c m ' ) in the Si overlayer. Consequently, new methods of defect reduction which inhibited defect formation during implantation were sought. Because the exact mechanisms of defect formation are still under investigation, many methods of defect reduction have been explored. Various techniques which reduce the defect density to as low as 10 cm' are discussed below.
1.3.1 Channeled Implants
1.3.2 Si Epitaxial Growth on S1MOX Substrates
An alternative method of fabricating a Si overlayer with a reduced defect density utilises the growth of a Si epitaxial layer on annealed SIMOX material. Figure 1.11 shows the reduction in dislocation density obtained as a function of Si epitaxial layer thickness. Though it is apparent that an order of magnitude reduction in dislocation density was achieved after epitaxial Si growth, this technique adds an extra processing step without significantly reducing the defect density. As well, the additional Si overlayer thickness is not compatible with the requirements for fully-depleted circuits. Still, in the mid-1980s it was a commonly utilised technique. Today, Si epitaxial layers are grown on SIMOX wafers when a thicker Si overlayer is required for specific applications such as three-dimensional circuits or high-power applications.34
DISTANCE ABOVE B U R I E D OXIDE ( p m )
1.3.3 Cavity Nucleation in the Si Overlayer
Under certain implantation conditions, high densities o f cavities (vacancy clusters) within the Si overlayer can result. During subsequent annealing these cavities act as stress-free sinks for O and Si interstitials, limiting the generation o f dislocation loops and confining such loops to regions near the buried oxide. These cavities are believed to be stabilised by O which forms a thin S i0 2 layer on the cavity walls and consequently, these cavities are stable up to temperatures o f ~1100°C. Annealing above
this temperature dissolves the cavities leaving a Si overlayer with a reduced defect density. (A defect density o f <104 cm*2 was reported using this method.)35 Unfortunately, cavities can only be produced with implant temperatures o f >600°C and high current densities. ’ Such implant conditions result in surface roughness and a poor quality buried oxide. Consequently, this technique is not used in production.
A similar method involving cavity nucleation through a 900°C, 0.5 hour has been reported.39*41 This technique combines sequential implantation and annealing (section 1.3.4) whereby the total dose (O) is reached through incremental implants o f ~ 0 /3 , for example. By annealing between implants at the low temperature o f 900°C (as compared to the final 1300°C anneal), strain within the Si overlayer is relieved and consequently dislocation nucleation occurs at higher total doses than without the intermediate annealing steps.
1.3.4 Multiple Implantation and Annealing
A significant advance in dislocation density reduction was made in 1988 when a threshold for dislocation formation in O-implanted Si was reported.42 At an implant energy o f 150 keV, the critical dose (<|>c) for dislocation formation was ~ 5 x l0 17 O/cm2. (The implant temperature for this work was not reported.) The three possible suggestions for the existence o f a threshold dose offered w ere:18 (1) the existence o f a critical O precipitate size above which dislocation loop formation resulted, (2) damage accumulation with increasing dose and (3) the accumulation o f tensile strain with increasing dose.
4x1017 O/cm2 and an intermediate annealing step at 1250°C for 17 hours had a final dislocation density of ~105 cm'2.19,43 Presently, dislocation densities acceptable for device fabrication (~10 cm’ ) are routinely achieved in SIMOX material produced using multiple implantation and annealing. The disadvantages of this technique include long anneals at high temperature which can result in wafer contamination and a higher cost per wafer due to the extra processing step(s).
1.3.5 Low-dose, Low-energy SIMOX
In 1991, the first report of low-energy, low-dose SIMOX material was published.44 The advantages of this technique include lower implant times (reduced fabrication costs), high quality Si device layers (the lower dose yields less damage during implantation), and an abrupt Si/Si02 interface due to the decreased straggling of the implanted ions. Various authors demonstrated SIMOX formation between 30-90 keV and doses of 1.5-3x1017 O/cm2, with very low defect densities45’47 In general, these SOI films are used only for fully-depleted devices. Given the advantages of this technique, extensive process optimisation is currently being pursued.
1.4 Scope of the present work
A variety of methods for producing SOI material have been reviewed. Presently, the most mature of these technologies is the SIMOX technique. Several methods of SIMOX material production resulting in a low-defect-density Si overlayer were presented. However, a complete understanding of the formation of dislocations within the Si overlayer has not been achieved. Further refinements to the SIMOX process as well as a more economical production of SIMOX material require a better understanding of the mechanisms of dislocation formation.
substrate cost. It also makes the exploration of low-temperature SIMOX material production possible. Such investigations are presented in Chapter 3.
Secondly, by virtue of the extended ion range, the damage at the ion end-of-range and within the Si overlayer are spatially separated, making it easier to study dislocation formation mechanisms in these two regions. The measurement of strain was used to indirectly study point defect types and interactions within high-energy O-implanted Si. Samples fabricated at various doses and implant temperatures were examined in order to gain a greater understanding of dislocation formation on an atomic scale in this material. The primary experimental tools utilised were double crystal x-ray diffraction (a very sensitive technique for studying strain in ion-implanted layers) and transmission electron microscopy to study defect microstructures. A discussion of strain accumulation and relief in relation to dislocation formation is presented in Chapter 4.
This chapter is divided into two parts, sample preparation and sample characterisation. Samples were fabricated using a high-current, high-energy ion implanter in conjunction with high-temperature annealing. Characterisation was performed with a variety of analytical techniques including Rutherford backscattering/channeling (RBS/C), transmission electron microscopy (TEM), double crystal x-ray diffraction (DCXRD) and variable-energy positron annihilation spectroscopy (VEP). The descriptions in the following sections are necessarily brief and a basic familiarity with some of these techniques is assumed.
2.1 Sample preparation
2.LI Ion Implanter
-negative ion source magnet
.focussing and steering
injection energy, approx. lOOkeV'"
servicing position tank
post acceleration energy:0.5-5.0 MeV
high voltage terminal magnet
control console apertures
type wherein positive Cs ions are attracted toward a negatively-biased Cu cathode filled with a powdered source of the element to be implanted. For instance, powdered Al20 3/Ag (1:1 by volume) and Si are the source materials for O and Si ions, respectively. Sputtered negative ions are accelerated through a potential difference (V0) of magnitude < 100 kV and thereafter exit the ion source.
A 90° magnet is then utilised for mass-filtering. If the Lorentz force on a charged particle (E = nqy x B) is set equal to the centrifugal force on the ion as it is deflected through a radius (R), the strength of the magnetic field (B) required for the desired mass (m) is:
where V = accelerating potential, n = ion charge state and q = electron charge. Typical O and Si ion beam currents achievable after mass filtering were -150 pA.
The tank depicted in Fig. 2.1 contains a 1.7 MV tandem accelerator. The high voltage terminal gains a high potential by the accumulation of positive charge; a moving chain of metal pellets connected by insulating links transports positive charge drawn from ground to the high voltage terminal. The voltage is sustained through a series of equipotential rings. The desired voltage is maintained by a series of corona points which leak off any additional charge.
The negative ions are injected into the accelerator and accelerated towards the positive terminal. There they are partially stripped of electrons in a gaseous charge exchange cell to become positively charged and are subsequently further accelerated away from the terminal as positive ions. The final ion energy is:
(assuming the ions are monatomic, i.e. not molecular) where n = the charge state of the ion. Ion can be accelerated to -0.2 to 10 MeV, where the maximum achievable energy is limited by the maximum attainable charge state of a given ion. If no stripping gas is used, negative ions are accelerated then decelerated through the terminal potential, emerging with the initial injection energy. The reader is referred to Rosenblatt48 for a more complete description of the operation of a tandem accelerator. Finally, a second electromagnet is utilised for energy filtering and then the ion beam is electrostatically scanned over an area-defining aperture situated -30 cm from the sample.
The target holder consists of a four-sided block of Cu or Ni with vertical translation and rotation capabilities. The sample is clamped to the block in as many
places as possible and, unless otherwise noted, conductive Ag paint is used to establish better thermal contact between the sample and target holder. A cartridge lodged inside the target holder provides heating. Alternatively, the target holder can be cooled with liquid nitrogen. An embedded k-type thermocouple measures the block temperature. Implant temperatures quoted in this thesis are the temperature of the target holder. Estimates of the error in sample temperature are discussed below.
Accurate dosimetry is determined with a capacitative-based charge integrator. Secondary electron emission is suppressed by a Cu cage maintained at -300 V that surrounds the target holder. In addition, the cage is cooled by liquid nitrogen to improve the local vacuum. The sample holder is electrically isolated from the suppression shield and ground. To minimise contamination due to the cracking of residual hydrocarbons on the sample surface, the pressure in the sample chamber was maintained at <5x1 O'7 Torr during implantation. The aperture defining the implantation area is made of Si to minimise contamination resulting from sputtering.
High-energy implants are susceptible to temperature rises due to the high power of the incident ion beam. The sample temperature is determined by the input power of the ion beam, the radiative heat losses at the sample surface and conductive heat transfer to the target holder. It has been shown49 that in the absence of conductive heat losses and with a beam power of 1.6 Watts/cm , the equilibrium wafer temperature is reached within 45 seconds, i.e. instantaneously as compared to the duration of a high-dose implant. In the present work, good thermal contact was made between the sample and target holder by utilising Ag paint on the backside of the wafer in addition to clamping. After the equilibrium temperature has been reached, the wafer temperature can be calculated by setting the ion beam power equal to the radiative heat losses plus the conductive heat transfer. If good thermal contact between the sample and the target holder is achieved, conductive heat losses will be limited by the thermal conductivity of Si. Thus, the wafer temperature can be calculated:
where Pb = power of the incident ion beam, A = area of implantation, a = Stefan-Boltzman constant (5.67x10* W/cm-K ), e = emissivity of the target
(0.35), Tw = wafer temperature, Tsurr = temperature of the surroundings, k = thermal conductivity of the wafer (~1 W/cm-K for Si), T ^ = target holder temperature and x = wafer thickness (0.035 cm). Tsurr was taken to be -150°C due to the temperature of the cold shield that surrounds the target holder. T ^ is the temperature measured by the thermocouple embedded into the target holder.
^ = 2oe(T4 - T « „ ) + A
utilised in this work, the conductive heat transfer to the target holder dominates. Equation 2.3 predicts that heat conduction through the wafer is such that the sample temperature does not exceed 1°C more than the target holder temperature even with a 20 W/cm ion beam. In the absence of conductive heat transfer, equation 2.3 predicts that an input power of 10 W/cm2 would result in an equilibrium sample temperature of ~973°C. However, clamping of the sample to the target holder even without Ag paint results in conductive heat transfer so the actual sample temperature will be much less than 973°C. The use of Ag paint will increase heat transfer and result in better temperature control and hence, a lower sample temperature.
An in-situ optical pyrometer could have yielded a more accurate measurement of the Si wafer temperature during implantation. That technique was unavailable so estimates of the implant temperature error were attained by studying the damage and strain within the Si overlayer with changes in the implant temperature. As shown in subsequent chapters, damage and strain within the Si overlayer of unannealed SIMOX material are strongly dependent on implant temperature. Consequently, RBS/C and strain measurements were used as an indicator of Si overlayer damage and hence implant temperature. Variations in the ion beam power for a given O dose did not affect the amount of damage and strain at implant temperatures of 300 or 450°C. Temperature control is consequently assumed to be good at implant temperatures of 300 and 450°C. At 150°C, the damage significantly increased with ion beam power, as expected, but never reached the same level as observed after 300°C implantation. Either the increased ion beam power resulted in an increased wafer temperature, or dose rate effects were observed. Because the ion beam power is so high, we are probably observing the effect of increased sample temperature. Based on strain measurements and the accurate temperature control that was observed with 300°C implantation, the actual temperature for 150°C implantation is assumed to be much less than 300°C.
2.1.2 Furnace Annealing
A Lindberg single-zone furnace equipped with an A120 3 tube was used for annealing. Annealing of O-implanted Si in an non-oxidizing ambient or in vacuum has been shown to produce severe pitting of the Si due to the formation of volatile SiO at the surface.50 The formation of SiO is favoured over Si02 at O partial pressures below 1 Torr at 1350°C.51 Thus, annealing is generally performed in an oxidizing ambient with or without a Si02 capping layer. The use of a Si02 capping layer minimises the consumption of Si during the annealing/oxidation process.
Chemical Vapour Deposition (PECVD) or via Spin-on-Glass (SOG). With a sufficiently thick capping layer (5000 Ä), Si consumption from the overlayer was minimised. Samples were annealed in 1-3% O in Ar. These concentrations of O are sufficiently high to prevent pitting of the surface and, in the absence of a capping layer, resulted in an Si02 layer thickness of 2000
A- 4000 Ä thick (consuming -950-1800
Aof the Si overlayer).
2.2 Sample Characterisation
2.2.1 Rutherford Backscattering
With the RBS technique, a beam of monoenergetic light ions impinges on the target to be analysed. The energy distribution of backscattered ions is subsequently measured and the depth distribution of the target constituents can be determined. The target can be oriented such that incident beam is aligned with a low index crystallographic direction such that a large portion of the incident beam is effectively “channeled” into the crystal by collisions with the regularly spaced lattice atoms. If the beam is oriented so that it is not aligned with any particular crystallographic direction (i.e. in a random orientation), channeling is inhibited. Channeled ions penetrate further into a crystal with less energy loss and fewer major interactions than occur for ions of random incidence. When channeled incident ions encounter damage in the target, the rate of dechanneling is increased and consequently the contribution of the random component to the backscattered ion yield is increased. The yield will be increased according to the structure and the magnitude of the disorder. Hence, channeling measurements can provide information on the depth distribution of disorder. The channeling minimum yield (Xmin) l s the ratio ° f the yields in a channeled orientation to a random orientation and can be used as a qualitative measure of crystal quality.
Hass Analyzer (25° magnet)
x it y steerer
Van de Graaf accelerator
[ <---- turbomoiecular pump
Collimator box (aperatures)
voltage drop to ground. The tank housing the terminal and column contains an insulting gas, in this case a N2/C 02 mixture, to prevent discharge of the high voltage terminal.
A Au-surface barrier (Schottky barrier) detector at a scattering angle of 168° (unless otherwise noted) detects backscattered particles. When particles impinge on the detector, electrons and holes are created and swept out of a depleted region. The resulting current pulse is proportional to the energy of the backscattered particle. The current/voltage pulse is routed through a pre-amplifier (amplification and pulse shaping) and amplifier (amplification and pulse shape analysis) to a multi-channel analyser (MCA). The MCA has 512 channels with a calibration of keV/channel.
2.2.2 Transmission Electron Microscopy
Another method of identifying damage in ion-implanted samples is Transmission Electron Microscopy (TEM). If the kinetic energy gained by an electron accelerated through a potential difference V, is set equal to the de Broglie equation relating wavelength and momentum, the electron wavelength (X) is:
2m0qV 1 + qV 2m0c
where m0 is the mass of an electron and c is the speed of light. With an accelerating voltage of 200 kV, the electron wavelength is 0.025 Ä. Since interatomic spacings are of the order of Ä, electrons make an ideal "probe" for imaging atoms.
objective lens x 25 intermediate lens x 8 projector lensx 100
Electron s o u r c e
C o n d e n s e r l ens
Objective l e n s <fca
— Focal p l a n e of obj ec t i ve -— y Selector a p e r t u r e
1 st. I nt er medi a t e I m a g e !•
I n t e r me d i a t e l e n s
\w / ■'/
V ' 2 n d I n t e r me d . a t e \ I m a g e / 2
Diffraction Mi croscopy
accelerated through a potential difference towards ground. Contrast in a specimen arises from phase and diffraction contrast.
A TEM can be used in various modes. A bright field image results when only the transmitted beam is used to form the image, with the objective aperture prohibiting a diffracted electron contribution to the final image. Hence, only the direct beam (and any low-angle inelastically scattered electrons) forms the specimen image. If the objective aperture is aligned with a diffracted beam, a dark field image is produced. Bright areas on the dark field image result from features that satisfy the Bragg condition for the diffracted beam orientation. Finally, the sample can be tilted in both the x and y planes to orient the beam along a given crystallographic direction. For the majority of the microscopy presented in this work, the sample was oriented in the  direction, then tilted 2° off-axis for enhanced contrast. The reader is referred to Hirsch, et al for a thorough description of TEM operation.
2.2.2b Sample Preparation for Cross-Sectional TEM (XTEM)
To view a specimen with TEM, the region of interest must be sufficiently thin for electron transmission. Electron transparency is dependent on a number of parameters such as the electron scattering factor (which increases with atomic number), the number of electrons scattered off the electron-optical axis, and the orientation of crystalline material. The minimum thickness for electron transparency at an accelerating voltage of 100 kV varies from several microns in Al to ~0.1 pm in U.
Ar ion gun
H Implanted area 20 um
Epoxy and sample surfaces
Figure 2.4: X T EM sample preparation steps: (a) Implanted faces glued together and mechanically polished, (b) sample after dimpling, (c) ion beam thinning o f the sample.
2.2.3 Double Crystal X-Ray Diffraction (DCXRD)
DCXRD analysis is a non-destructive technique widely used for compositional and structural analysis o f thin films. It can be utilised to obtain a quantitative measurement o f lattice strain which is measurable to 1 part per million (ppm). By comparison with theoretical rocking curves (RCs), depth distributions o f lattice strain can be obtained.
Figure 2.6 shows the experimental arrangement o f a double crystal diffraction system. A Bede QC2a diffractometer functioning in a (+,-) non-dispersive parallel arrangement (identical crystals for the reference and sample crystal, which are arranged
anti-parallel to each other) was used in this work. Cu x-rays are incident on a reference crystal o f the same material and orienatation as the sample. The reference crystal acts as a monochromator, removing the wavelength dispersion inherent in an x-ray source. X-rays are diffracted when the incident angle 0, is equal to the Bragg
angle. The Bragg condition is:
nX = 2dsin0B (2.5)
while a scintillation detector measures the diffracted x-ray intensity. Because the specimen and reference crystal are parallel, only x-rays satisfying the Bragg condition for both crystals reach the detector. The extinction depth (the depth at which the x-ray intensity falls to 1/e of the initial intensity) is given by:
Le = - V s i n 9 B (2.6)
where rc = classical electron radius, Fh = real part of the structure factor and Vc = volume of the unit cell.53 For Cu K« radiation incident on (004) Si at the Bragg angle, Lc = 4.82 pm.
The sample is "rocked" through some angle co, by tilting the sample as indicated in Figure 2.5. The detector is simultaneously moved through an angle 2co and the diffracted x-ray intensity as a function of detector angle is recorded. A substrate peak as well as satellite peaks from any variations in lattice spacing due to mismatch, strain and/or compositional differences appear in the spectra when w=0B. The differential form of Bragg's law relates the strain and therefore the difference in lattice parameter between the layer and substrate to the angular separation Aw, of the their Bragg peaks:
— = (-cote)Am. (2.7)
Peaks to the right of the substrate peak are due to a lattice contraction (tensile strain) while peaks to the left of the substrate peak are due to lattice expansion (compressive strain). In ion-implanted material, the angular separation between peaks is determined by the difference in lattice spacing between the implanted layer and substrate. The intensity and width of the diffraction peak is related to the thickness, depth, composition and structural damage of the strained layer.
For thin epitaxial layers, fringes appear in the RC which can be used to calculate layer thicknesses. Each layer will give rise to a specific periodicity in the rocking curve. This characteristic period (A0) is given by:
Reference Crystal Si (400) /
Figure 2.5: Schematic o f a double crystal x-ray diffractometer.
2.2.3a Depth Distribution o f Strain in Ion-implanted Material
Several models for the evaluation o f strain in ion-implanted material have been reported (see Table I). Typically, the strain depth distribution is modeled after the displaced atom distribution. It has been reported that strain due to interstitials is an order o f magnitude higher than that due to vacancies/ Indeed, Pesek, et al noted that the strain profile in Ge-implanted Si was proportional to a linear combination o f the damage and ion distributions; at low doses, the strain was proportional to the damage distribution while at high doses it was proportional to the ion distribution. More recently, a fitting procedure for RC analysis in ion-implanted semiconductors was reported wherein strain caused by implantation-induced vacancies was neglected due to
58 the aforementioned studies.
Under common experimental conditions (room temperature and a dose o f
A u th o r M a te ria ls sy stem M o d e le d strain d istrib u tio n
C o m m e n ts
M a c N e a l et a l62 N e ,B ,H e -im p la n te d oc d a m a g e ( n u c le a r sig n a l d is a p p e a re d
m a g n e tic b u b b le d is p la c e m e n ts ) u p o n a m o rp h o u s la y e r
g a rn e t m a te ria ls d istrib u tio n * ion
d istrib u tio n
fo rm a tio n
P e se k et a l57 G e -im p la n te d Si x d a m a g e (n u c le a r
d is p la c e m e n ts ) d istrib u tio n * ion d istrib u tio n
-S e rv id o ri59 S i-im p la n te d Si x d is p la c e d a to m
d e n s ity
n e g a tiv e strain
a p p e a re d a fte r o n s e t o f a m o rp h is a tio n
P a in e e t a l63’64 H e ,B ,C ,N e ,S i,P ,T e -i x e n e rg y d e p o s ite d
m p la n te d G aA s in to n u c le a r c o llisio n s
-H a rt e t al65 S i,A r-im p la n te d Si x d is p la c e d a to m
d e n s ity
B e rti et a l66 N -im p la n te d Si x d is p la c e d a to m
d e n s ity (c o rre la te d w ith R B S /C m e a s u re m e n ts )
a re a u n d e r th e (D C X R D ) stra in p e a k sa tu ra te d a fte r a m o rp h is a tio n
B ai et al67 S i-im p la n te d Si x d is p la c e d ato m
d e n s ity
F a b b ri et al61 B ,G e -im p la n te d Si x d isp la c e d ato m
p ro file a n d la ttic e e x p a n s io n /c o n tra c tio n d u e to im p la n te d ion su b stitu tio n a lity
n e g a tiv e a n d p o sitiv e stra in e v id e n t at all d o se s
E llin g b o e et a l68 0 , S i-im p la n te d Si x im p la n ta tio n -in d u c e d
v a c a n c y e x c e s s d e p th p ro file
o n ly n e g a tiv e strain e v id e n t (all sa m p le s h a d an a m o rp h o u s la y e r at R,,)
V e n a b le s et a l39 O -im p la n te d Si x e x c e s s p o in t d e fe c t
p ro file
p o s itiv e stra in at low d o se s a n d n e g a tiv e stra in at h ig h d o se s
Z h o u e t a l69 0 - im p la n te d Si x v a c a n c y -ric h re g io n
a h e a d o f 0 io n e n d o f ra n g e
n e g a tiv e strain e v id e n t, o n ly h ig h d o s e s re p o rte d ( > 8 x l 0 17 cm*2)
Table I: Reports o f strain models in ion-implanted material.
vacancy-type defects at lesser depths. (It is assumed the implant temperature is high enough to reduce the number of displaced atoms in the surface layer such that the point defect profile in this region is dominated by vacancy-type defects.)
2.2.3b Rocking Curve Analysis by Dynamical Simulation (RADS)
Simulations of RCs in this work were performed with the software package RADS which uses the solution of the Takagi-Taupin equations • of dynamical theory for the analysis of strain in epitaxial thin films. Trial strain distributions (based on implantation parameters, TRIM90 simulated point defect depth distributions and XTEM analysis) are iteratively entered into RADS until a reasonable agreement between theory and experiment results. Given the depth-dependent defect distribution in ion-implanted material, the interpretation of RCs from ion-implanted material is difficult. In addition, the diffuse scattering of x-rays (Huang scattering) due to implantation-induced extended defects can greatly influence the calculated strain profile.74 Typical RCs have a high background signal from the extended defect formation. Furthermore, complex strain profiles must be modeled RADS as thin layers of discrete strain levels. However, changes in strain with implanted dose and/or temperature variations are readily apparent from RADS simulations and the peak strain can also be accurately determined.
2.2.3c Strain depth profiling in ion implanted material
Implant Energy (keV)
Dose (Si/cm2) Depth of amorphisation (pm)'
100 5xl015 0.2
300 5xl015 0.65
600 5xl015 1.05
* as obtained by RBS/C measurements.
Table II: Implant parameters o f Si implant amorphisations.
1 7 - 2 The sample used for this study was O-implanted Si (1 MeV, 7x10 cm’ , 225°C), where the numbers in parentheses refer to the implant energy, implant dose and the implant temperature, respectively. This format of describing implant parameters will be used henceforth to ease in the reading of this thesis. The experimental and simulated RC for this sample are shown in Figure 2.6. The inset shows the strain profile used in the RADS simulation. In Figure 2.7, the RC for the same sample but after amorphisation to 0.2 pm is pictured. Again, the inset shows the same simulation used as in Figure 2.6 but with the strain in the implantation-induced amorphous layer set equal to zero. A close fit between experiment and simulation results in both cases indicating that the strain peak at -100 arcsec in Fig. 2.6 was due to strain in the top 0.2 pm of the Si. After amorphising the sample even further to 0.6 pm and setting the strain to zero in the RADS simulation over this depth, a good fit between the simulated and experimental RCs again results (Figure 2.8). No secondary strain peaks were evident in the RC for the sample amorphised to 1.05 pm (not shown) indicating that all of the strain was contained in the first 1.05 pm i.e. in the Si overlayer.
0.7x1018 O /cm 2, experimental RADS simulation
- 3 0 0 0
^ - 2 5 0 °
q. - 2 0 0 0
w - 1 5 0 0
o -1 0 0 0
05 - 5 0 0
0.0 0.2 0.4 0.6 0 .8 1.0 1.2
Depth (/xm )
- 5 0 01 0 0 0
T h e t a / 2 T h e t o (A r c se c )
I I I I ' 1 ' ' I
0 .7 x l0 18 O/cm2 + amorphisation to 0.2 pm RADS simulation
0.0 0.2 0.4 0.6 0.8 1.0 1.2
- 5 0 0 0 5 0 0
T h e ta /2 T h e ta (Arcsec)
Figure 2.7: DCXRD spectra for the O-implanted Si sample (1 MeV,
I I I I I I r
0.7x1018 O /cm 2 + amorphisation to 0.6 pm RADS simulation
- 5 0 0 0 500 1000
Th e t a /2 T h e t a (Arcsec)
Figure 2.8: DCXRD spectra for the O-implanted sample (1 MeV,
2.2.4 Variable Energy Positron Annihilation Spectroscopy (VEP)
Energetic positrons incident on a solid will rapidly thermalise upon contact and diffuse through the solid. After spending the majority of their lifetime in this freely diffusing state, positrons will annihilate with electrons in the solid. The probability of a positron annihilating with an electron from a given momentum state is determined by the overlap of its wave function. The annihilation y-rays emitted will be Doppler- broadened about the mean energy of 511 keV due additional electron momentum (or energy). The y-ray distribution can be measured directly using the angular correlation of the annihilation radiation (ACAR) technique but it is more common to employ Doppler-broadening spectroscopy which is faster and more economical.75,76 (The latter technique was used in this work.)
Thermalised positrons have a high probability for capture and annihilation in open volume (i.e. vacancy-type) defects.77 When an open-volume defect is encountered by a diffusing positron, the positron will rapidly (~10’15 sec) be localised by the defect. Trapping of the positron results in the overlap of the positron wave function with the core electrons to either be reduced (vacancies) or increased (impurities) and the lineshape of the y-ray distribution is accordingly narrowed or broadened. The annihilation lineshape is usually characterised by an S (".Sharpness") or W ("fFidth") parameter. The definition of these parameters is illustrated in Figure 2.9 and the specific y-ray energies over which the W and S parameters were measured is stated. The response of the positron wave function in different trap environments and the corresponding change in lineshape parameters is illustrated in Figure 2.10. The S-parameter increases as the lineshape becomes narrower while the W-parameter increases as the lineshape broadens. With the use of variable energy positrons, the probing depth may be varied and the vacancy and/or impurity-type defect depth distribution subsequently derived. This technique has been successful in studying ion-implanted Si78'80 and the Si/Si02 interface.81
Modeling programs are available to aid in data interpretation and deduce whether annihilation has occurred from either a freely diffusing positron, trapping at the surface or trapping by a point defect. Without any guidance in the fitting procedure, there is any number of solutions. The models used in this work therefore involved a systematic study of different samples and fixing of parameters such as layer depth (which was obtained using other techniques such as XTEM or RBS). The VEP measurements reported in this work were performed by P.J. Schultz and co-workers at
Total Peak: integrated from 504.5 - 517.5 keV
504.5 keV 511 keV 517.5 keV
over: 510.1 - 511.9 keV
B] + B2
is integrated over: 507.7 - 509.5 keV
is integrated over: 512.5-514.5 keV
Figure 2.9: A definition o f lineshape parameters, S and W.
Trap "A" ( o p e n v o l u m e )
© © © © ©
© © © © ©
Fr e e Anni hi l at i on
Trap "8" ( i mpur i t y )
© © © © ©
© © © ©
SIMOX Substrate Formation by High-Energy
As noted previously, “conventional” SIMOX substrates are typically formed by
200 keV O implantation in Si to a dose of 1.4x10 cm' . At this dose, stoichiometric Si02 is formed during implantation when the peak of the O depth distribution reaches 67 atomic %. During implantation, the substrate is maintained at ~600°C to inhibit amorphisation of the Si overlayer. A post-implant anneal at high temperature (~1300°C for 4 hours) is necessary to induce O segregation from substoichiometric depths and reduce lattice disorder. If a thicker overlayer is required, an epitaxial Si layer is subsequently grown by chemical vapour deposition.
achieve stoichiometry during implantation. From TRIM90 simulations, the ion dose must be increased by a factor of -1.5 to achieve stoichiometry when the energy is increased from 200 to 1000 keV.
To date, the author is unaware of any report of MeV O-ion implantation in Si to stoichiometric doses though several groups have investigated SIMOX substrate fabrication with sub-stoichiometric doses. ’ In the earliest report of sub-stoichiometric MeV O-ion implantation, White et al50 found that buried Si02 layers from high-energy implants formed in essentially the same way as those from low-energy implants, i.e. implant temperature was the most crucial parameter in forming a uniform buried Si02 layer. At implant temperatures >400°C, O segregated into Si02 precipitates prematurely and impeded the formation of a uniform buried oxide layer. Low implant temperatures resulted in more uniform buried Si02 layers and the formation of polycrystalline or twinned Si at the front amorphous/crystalline (a/c) interface, depending on the annealing conditions.
In 1988, Nieh et al reported 2 and 5 MeV sub-stoichiometric O-ion implantation at -197, 20 and 500°C. This was the first report of MeV, high dose O-implanted Si at and below room temperature. In such material, the defect density in the Si overlayer after a 1300°C anneal was estimated to be -10 cm' , comparable to that observed in single implant and anneal SIMOX fabricated at 200 keV implant energies at a temperature of 500°C.
In this chapter, the formation of a Si02 layer by 1 MeV O-ion implantation to stoichiometric doses is presented. The dose, implant and annealing temperature dependencies of both defect evolution in the Si overlayer and the formation of a buried Si02 layer are described. The results of Si-ion implantation, performed under similar conditions to those used for the O implantation, are then presented with the aim of elucidating any chemical effects relevant to damage formation in SIMOX material.
3.1 High-Energy O-ion Implantation
3.1.1 Dependence o f Damage on O Dose
1 MeV 2 0 0 keV
D e p th Oxm)
Figure 3.1: Calculated vacancy (— ) and O atom (——) depth distribution at 200 and 1000 keV for doses o f 1.4xl018 and 2.15xl018 O/cm2,
2.15x10 O/cm at 200 keV and 1 MeV, respectively) are those necessary to achieve stoichiometry during implantation. The predicted vacancy concentration at the surface is lower for 1 MeV implantation, indicating that less damage within the Si overlayer results from implantation at higher implant energies.
Yield corresponding to
Figure 3.2: RBS/C spectra (obtained with 3 M eV He+ ions) fo r a 450°C
implant at various O doses: (a) 0.73xl018, (b) 1.45xl018, (c) 2.1 8 xl0 18 and
j o y
(d) 2.64x10 cm . The detector was at a scattering angle o f 120°.